Structure determination of KScS~2~, RbScS~2~ and KLnS~2~ (Ln = Nd, Sm, Tb, Dy, Ho, Er, Tm and Yb) and crystal‒chemical discussion
Havlák, Lubomír; Fábry, Jan; Henriques, Margarida; Dušek, Michal; Acta Crystallographica Section C 71 (2015) 623–630; doi:10.1107/S2053229615011833

data_2020012
_publ_section_title
;
 Structure determination of KScS~2~, RbScS~2~ and KLnS~2~ (Ln = Nd, Sm,
 Tb, Dy, Ho, Er, Tm and Yb) and crystal--chemical discussion
;
_journal_coeditor_code           FA3364
_journal_issue                   7
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              623
_journal_page_last               630
_journal_paper_doi               10.1107/S2053229615011833
_journal_volume                  71
_journal_year                    2015
_chemical_formula_iupac          'K1 Dy1 S2'
_chemical_formula_moiety         'Dy1 K1 S2'
_chemical_formula_sum            'Dy K S2'
_chemical_formula_weight         265.7
_chemical_name_systematic
;
Potassium dysprosium sulfide
;
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   4.0315(11)
_cell_length_b                   4.0315(11)
_cell_length_c                   21.890(5)
_cell_measurement_reflns_used    386
_cell_measurement_temperature    293.5(6)
_cell_measurement_theta_max      28.62
_cell_measurement_theta_min      5.89
_cell_volume                     308.11(14)
_computing_cell_refinement
;
<i>CrysAlis PRO</i> (Agilent, 2014)
;
_computing_data_collection
;
<i>CrysAlis PRO</i> (Agilent, 2014)
;
_computing_data_reduction
;
<i>CrysAlis PRO</i> (Agilent, 2014)
;
_computing_publication_material
;
<i>JANA2006</i> (Pet\<r\'i\<cek <i>et al.</i>, 2014)
;
_computing_structure_refinement
;
<i>JANA2006</i> (Pet\<r\'i\<cek <i>et al.</i>, 2014)
;
_computing_structure_solution
;
SUPERFLIP (Palatinus & Chapuis, 2007)
;
_diffrn_ambient_temperature      293.5
_diffrn_detector_area_resol_mean 5.1873
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.93
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type
'Xcalibur Gemini Ultra diffractometer with Atlas detector'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0995
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -3
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            658
_diffrn_reflns_theta_full        27.76
_diffrn_reflns_theta_max         29.26
_diffrn_reflns_theta_min         5.59
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    19.974
_exptl_absorpt_correction_T_max  0.7034
_exptl_absorpt_correction_T_min  0.2009
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
<i>JANA2006</i> (Pet\<r\'i\<cek <i>et al.</i>, 2014)
;
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    4.2962
_exptl_crystal_description       block
_exptl_crystal_F_000             351
_exptl_crystal_size_max          0.208
_exptl_crystal_size_mid          0.085
_exptl_crystal_size_min          0.031
_refine_diff_density_max         4.44
_refine_diff_density_min         -2.46
_refine_ls_extinction_coef       19E2(4)
_refine_ls_extinction_method
;
B-C type 1 Lorentzian isotropic
[Becker, P. J. & Coppens, P. (1974). <i>Acta Cryst.</i> A<b>30</b>, 129--147]
;
_refine_ls_goodness_of_fit_ref   2.32
_refine_ls_number_constraints    0
_refine_ls_number_parameters     9
_refine_ls_number_reflns         126
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0519
_refine_ls_R_factor_gt           0.0516
_refine_ls_shift/su_max          0.0011
_refine_ls_shift/su_mean         0.0002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     'w = 1/[\s^2^(I) + 0.0004I^2^]'
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.1050
_refine_ls_wR_factor_ref         0.1050
_reflns_number_gt                124
_reflns_number_total             126
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            fa3364sup1.cif
_cod_data_source_block           VI
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_original_formula_sum        'Dy1 K1 S2'
_cod_database_code               2020012
_cod_database_fobs_code          2020012